LMucko/crystallography-open-database huggingface dataset:
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101678
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.25 O4 W Zn0.75'
_chemical_formula_weight         312.77
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                89.766(2)
_cell_angle_beta                 91.135(2)
_cell_angle_gamma                91.467(2)
_cell_formula_units_Z            2
_cell_length_a                   4.68499(11)
_cell_length_b                   5.73796(16)
_cell_length_c                   4.91163(12)
_cell_volume                     131.966(6)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           75
_cod_original_formula_sum        'Cu0.25 O4 W1 Zn0.75'
_cod_database_code               2101678
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101679
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.3 O4 W Zn0.7'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                89.6303(19)
_cell_angle_beta                 91.1899(18)
_cell_angle_gamma                92.0730(18)
_cell_formula_units_Z            2
_cell_length_a                   4.68411(10)
_cell_length_b                   5.74374(13)
_cell_length_c                   4.90925(10)
_cell_volume                     131.963(5)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           70
_cod_original_formula_sum        'Cu0.30 O4 W1 Zn0.70'
_cod_database_code               2101679
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101680
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.35 O4 W Zn0.65'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                89.3597(14)
_cell_angle_beta                 91.3394(13)
_cell_angle_gamma                93.2364(13)
_cell_formula_units_Z            2
_cell_length_a                   4.69010(10)
_cell_length_b                   5.76474(13)
_cell_length_c                   4.90647(8)
_cell_volume                     132.403(5)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           65
_cod_original_cell_volume        132.403(4)
_cod_original_formula_sum        'Cu0.35 O4 W1 Zn0.65'
_cod_database_code               2101680
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101681
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.4 O4 W Zn0.6'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                89.2071(13)
_cell_angle_beta                 91.4870(12)
_cell_angle_gamma                93.9239(13)
_cell_formula_units_Z            2
_cell_length_a                   4.69097(9)
_cell_length_b                   5.77510(9)
_cell_length_c                   4.90169(7)
_cell_volume                     132.425(4)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           60
_cod_original_formula_sum        'Cu0.40 O4 W1 Zn0.60'
_cod_database_code               2101681
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101682
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.45 O4 W Zn0.55'
_chemical_formula_weight         312.40
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                89.1685(17)
_cell_angle_beta                 91.5190(16)
_cell_angle_gamma                94.1000(16)
_cell_formula_units_Z            2
_cell_length_a                   4.69174(12)
_cell_length_b                   5.77857(13)
_cell_length_c                   4.90054(9)
_cell_volume                     132.464(5)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           55
_cod_original_formula_sum        'Cu0.45 O4 W1 Zn0.55'
_cod_database_code               2101682
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101683
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.55 O4 W Zn0.45'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.913(2)
_cell_angle_beta                 91.8172(19)
_cell_angle_gamma                95.215(2)
_cell_formula_units_Z            2
_cell_length_a                   4.69651(18)
_cell_length_b                   5.80159(18)
_cell_length_c                   4.89491(11)
_cell_volume                     132.736(7)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           45
_cod_original_cell_volume        132.733(8)
_cod_original_formula_sum        'Cu0.55 O4 W1 Zn0.45'
_cod_database_code               2101683
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101684
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.6 O4 W Zn0.4'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.871(3)
_cell_angle_beta                 91.828(3)
_cell_angle_gamma                95.367(3)
_cell_formula_units_Z            2
_cell_length_a                   4.6947(3)
_cell_length_b                   5.8028(3)
_cell_length_c                   4.89158(16)
_cell_volume                     132.588(12)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           40
_cod_original_cell_volume        132.588(11)
_cod_original_formula_sum        'Cu0.60 O4 W1 Zn0.40'
_cod_database_code               2101684
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101685
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.65 O4 W Zn0.35'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.706(2)
_cell_angle_beta                 92.051(2)
_cell_angle_gamma                95.982(2)
_cell_formula_units_Z            2
_cell_length_a                   4.70189(11)
_cell_length_b                   5.81866(18)
_cell_length_c                   4.89057(11)
_cell_volume                     132.962(6)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           35
_cod_original_cell_volume        132.962(8)
_cod_original_formula_sum        'Cu0.65 O4 W1 Zn0.35'
_cod_database_code               2101685
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101686
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.7 O4 W Zn0.3'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.678(4)
_cell_angle_beta                 92.073(4)
_cell_angle_gamma                96.099(4)
_cell_formula_units_Z            2
_cell_length_a                   4.7013(4)
_cell_length_b                   5.8207(4)
_cell_length_c                   4.8890(2)
_cell_volume                     132.918(16)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           30
_cod_original_cell_volume        132.917(16)
_cod_original_formula_sum        'Cu0.70 O4 W1 Zn0.30'
_cod_database_code               2101686
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101687
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.7 O4 W Zn0.25'
_chemical_formula_weight         311.86
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.5414(13)
_cell_angle_beta                 92.2845(12)
_cell_angle_gamma                96.6112(13)
_cell_formula_units_Z            2
_cell_length_a                   4.70508(13)
_cell_length_b                   5.82979(11)
_cell_length_c                   4.88441(7)
_cell_volume                     132.951(5)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           25
_cod_original_cell_volume        132.952(5)
_cod_original_formula_sum        'Cu0.70 O4 W1 Zn0.25'
_cod_database_code               2101687
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101688
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.8 O4 W Zn0.2'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.511(2)
_cell_angle_beta                 92.3254(17)
_cell_angle_gamma                96.7350(19)
_cell_formula_units_Z            2
_cell_length_a                   4.70707(19)
_cell_length_b                   5.83407(18)
_cell_length_c                   4.88649(10)
_cell_volume                     133.124(7)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           20
_cod_original_cell_volume        133.124(8)
_cod_original_formula_sum        'Cu0.80 O4 W1 Zn0.20'
_cod_database_code               2101688
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101689
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.85 O4 W Zn0.15'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.4601(12)
_cell_angle_beta                 92.3623(10)
_cell_angle_gamma                96.8837(11)
_cell_formula_units_Z            2
_cell_length_a                   4.70559(12)
_cell_length_b                   5.83597(10)
_cell_length_c                   4.88391(6)
_cell_volume                     133.008(4)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           15
_cod_original_cell_volume        133.008(5)
_cod_original_formula_sum        'Cu0.85 O4 W1 Zn0.15'
_cod_database_code               2101689
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101690
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.9 O4 W Zn0.1'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.413(2)
_cell_angle_beta                 92.5035(18)
_cell_angle_gamma                97.095(2)
_cell_formula_units_Z            2
_cell_length_a                   4.7095(2)
_cell_length_b                   5.8403(2)
_cell_length_c                   4.88323(11)
_cell_volume                     133.123(8)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           10
_cod_original_cell_volume        133.122(9)
_cod_original_formula_sum        'Cu0.90 O4 W1 Zn0.10'
_cod_database_code               2101690
Distortion Characteristics Across the Structural Phase Transition in (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
Schofield, P. F.; Knight, K. S.; Redfern, S. A. T.; Cressey, G.; Acta Crystallographica Section B 53 (1997) 102–112; doi:10.1107/S0108768196010403

data_2101691
_publ_section_title
;
 Distortion Characteristics Across the Structural Phase Transition in
 (Cu~1{-~<i>x</i>}Zn~<i>x~</i>)WO~4~
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              102
_journal_page_last               112
_journal_paper_doi               10.1107/S0108768196010403
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu0.95 O4 W Zn0.05'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                88.3889(11)
_cell_angle_beta                 92.4646(10)
_cell_angle_gamma                97.1148(10)
_cell_formula_units_Z            2
_cell_length_a                   4.70682(11)
_cell_length_b                   5.83985(10)
_cell_length_c                   4.88214(6)
_cell_volume                     133.004(4)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.227
_cod_data_source_file            ha0150.cif
_cod_data_source_block           5
_cod_original_cell_volume        133.004(5)
_cod_original_formula_sum        'Cu0.95 O4 W1 Zn0.05'
_cod_database_code               2101691